2Pozzolan The name Pozzolan comes from the town Pozzuoli, Italy. Ancient Romans (~100 B.C.) produced a hydraulic binder by mixing hydrated lime with soil (predominantly volcanic ash)Horasan mortar, mixing lime with finely divided burned clay, is extensively used by OttomansNowadays, the word pozzolan covers a broad range of natural and artificial materials.
3Pozzolana material that, when used in conjunction with portland cement, contributes to the properties of the hardened concrete through hydraulic or pozzolanic activity, or both.Natural (Volcanic ash, volcanic tuff, pumicite)Artificial (fly ash, silica-fume, granulated blast furnace slag)
4PozzolanSiliceous or aluminous material, which in itself possesses little or no cementitious value but will, in finely divided form and in the presence of moisture, chemically react with calcium hydroxide Ca(OH)2 to form compounds possessing hydraulic cementitious properties.
5POZZOLANIC REACTIONSCalcium Hydroxide+Silica+Water → “Calcium-Silicate-Hydrate”(C-S-H)C-S-H provides the hydraulic binding property of the material.Pozzolanic Activity: Capacity of pozzolan to form alumino-silicates with lime to form cementitious products. (How good how effective the pozzolan is!)
6FACTORS THAT AFFECT THE ACTIVITY OF POZZOLANS 1) SiO2 + Al2O3 + Fe2O3 content2) The degree of amourpheness of its structure3) Fineness of its particles
71) SiO2 + Al2O3 + Fe2O3The greater amount of these, the greater its activity.ASTM C 618 & TS 25 → min “SiO2+Al2O3+Fe2O3” for natural pozzolans > 70%Fly Ash - ASTMClass C→ from lignitide or subbituminous coals (SiO2+Al2O3+Fe2O3>50%)Class F→ from bituminous coals and SiO2+Al2O3+Fe2O3>70%Silica fume → SiO2 ≈ 85-98%Blast Furnace Slag→ SiO2 ~ 30-40%Al2O3 ~ 7-19%CaO ~ 30-50%
82) Amorphousness For chemical reaction → pozzolans must be amorphous Volcanic ash, volcanic tuff, fly ash, silica fume are all amorphous by nature.Clays → contain high amounts of silica & alumina but have a crystallic structure! (Do not possess pozzolanic activity)However, by heat treatment, such as calcining ~ °C crystallic structure is destroyed & a quasi-amorphous structure is obtained.
92) AmorphousnessClay → does not possess pozzolanic propertyBurned clay → possess pozzolanic propertyBlast furnace slag → contain high amounts of silica, alumina & lime.However, if molten slag is allowed to cool in air, it gains a crystal structure. * do not possess pozzolanic property.However, if it is cooled very rapidly by pouring it into water, it becomes a granular material & gains amorpousness. * possess pozzolanic property.
103) Fineness Pozzolanic activity increases as fineness increases. Volcanic ash, rice husk ash, fly ash, condensed silica fume are obtained in finely divided form.Volcanic tuff, granulated blast furnace slag & burned clay must be ground.
11DETERMINATION OF POZZOLANIC ACTIVITY Pozzolanic activity is determined by “strength activity indexes”Six mortar cubes are prepared (ASTM)→”Control Mixture” 500 g portland cement+1375 g sand+242 ml water→”Test Mixture” 400g of portland cement+100g of pozzolan+1375g of sand+some water for the same consistency
12Compressive testing at 7 or 28 days Strength Activity Index (SAI) =A/B*100A=f’c of test mixtureB=f’c of control mixtureASTM C 618 → SAI ≥ 75%
13CHEMICAL COMPOSITION OF POZZOLANS Silica Fume is mostly SiO2G. G. Blast Furnace Slag→ high amounts of CaO (self-cementitious)Class C Fly Ash has CaO (self-cementitious)
14Chemical Analysis of Typical Fly Ash, Slag, Silica Fume, Calcined Clay, Calcined Shale, and MetakaolinClass F fly ashClass C fly ashGroundslagSilica fumeCalcined clayCalcined shaleMeta-kaolinSiO2, %523590585053Al2O3, %2318120.4292043Fe2O3, %1161480.5CaO, %521401.60.1SO3, %0.84.19Na2O, %1.05.80.30.2—0.05K2O, %2.00.72.22Total Naeq. alk, %126.96.36.199.5Artificial PozzolansNatural PozzolansTable 3-2. Chemical Analysis and Selected Properties of Typical Fly Ash, Slag,Silica Fume, Calcined Clay, Calcined Shale, and Metakaolin
16Selected Properties of Typical Fly Ash, Slag, Silica Fume, Calcined Clay, Calcined Shale, and MetakaolinClass F fly ashClass C fly ashGroundslagSilica fumeCalcined clayCalcined shaleMeta-kaolinLoss on ignition, %2.80.51.03.01.50.7Blaine fineness, m2/kg42040020,00099073019,000Relative density2.382.652.942.402.502.63Table 3-2. Chemical Analysis and Selected Properties of Typical Fly Ash, Slag,Silica Fume, Calcined Clay, Calcined Shale, and Metakaolin
17Typical Amounts of Pozzolans in Concrete by Mass of Cementing Materials Fly ashClass C 15% to 40%Class F 15% to 20%Slag 30% to 45%Silica fume 5% to 10%Calcined clay 15% to 35%Metakaolin 10%Calcined shale 15% to 35%
18REQUIREMENTS FOR AN ACCEPTABLE QUALITY OF POZZOLAN TS 25 → Natural PozzolansTS 639 → Fly AshASTM C 618 → For Natural Pozzolan & Fly AshNaturalClass FClass CFineness (max. % retained when wet sieved on 45 mm sieve)34%Strength Activity Index75min "SiO2+Al2O3+Fe2O3"7050
19USES OF POZZOLANS1) Direct use of Pozzolan by Mixing it with Calcium HydroxideExtensively used in ancient times but not very common now.2) Use of Pozzolan in Producing Blended CementsGrinding “Clinker+Pozzolan+Gypsum”→ Portland Pozzolan Cements Extensively used3) Use of Pozzolan as an Admixture“Cement+Pozzolan+Aggregate+Water”→ Concrete